rom the Job-mix Formu on the Properties of Paving Mixtures
By Norman W. McLeod*
Substantial ranges of values for air voids, VMA, Marshall stability, and flow index, due to differences in paving mixture composition because of AASHTO and ASTM tolerances, have been demonstrated by this investi- gation. The portion of each of these ranges of values below and above similar values for the corresponding job-mix formula has been determined. It is shown that the single curves presently employed to illustrate design data for various paving mixture properties, such as air voids, VMA, etc., versus asphalt content, should be replaced by bands whose width depends primarily upon the tolerances being applied. ASTM and AASHTO tolerances have a drastic effect on filler/bitumen ratios, and on paving mixture pro- perties that are influenced by filler/bitumen ratios. The test data obtained demonstrate that the density of a paving mixture provided by its job-mix formula can fail by a substantial margin to represent the densities of other paving mixtures within the AASHTO and ASTM tolerance range. Con- sequently, the target density employed for controlling compaction by rolling in the field should ordinarily be provided by the laboratory compacted density determined on a sample of pavement taken at the precise location where the in-place density measurement was made. The test data tend to support end result specifications with realistic tolerances, and statistical quality control, wherein the contractor would assume full responsibility for the quality of paving operations, and would be subject to a graduated penalty scale for any section (lot) of pavement found to be off-specification.
Key Words: tolerances, job-mix formula, gradation, asphalt content, air voids, VMA, Marshall stability, flow index, particle index, filler/bitumen ratio, compaction control.
The job-mix formula for a hot-mix asphalt paving mixture must satisfy specification requirements, and provides or should provide, the following items of information:
1. a single grading curve 2. a single asphalt content in per cent by weight 3. a single VMA value 4. a single air voids value 5. a single Marshall stability rating in pounds at 140F 6. a single flow index measurement in units of 0.01 inch 7. a single value for 100 per cent laboratory compacted density
* Norman W. McLeod, Vice President and Asphalt Consultant, McAsphalt Engineering Services, Toronto, Ontario, Canada.
Canadian Technical Asphalt Association 1976
It is a physical impossibility for even the best operated and most closely controlled hot-mix plants to turn out batch after batch that will conform exactly to the value for each of the above seven basic items that are associated with the job-mix formula. Even if it were, the lack of sufficient precision in current sampling and testing procedures would result in some reported deviation from the job-mix formula. This is recognized in properly written specifications for asphalt concrete, and they therefore contain what are referred to as tolerances. Tolerances are the amounts or degrees by which a paving mixture is permitted to deviate from the job-mix formula and still be considered to be on-specification.
At the present time, even carefully written specifications ordinarily contain tolerances for only each of the first two of the above seven items, that is tolerances for permissible deviation away from the grading curve, and from the per cent asphalt content by weight stipulated by the job-mix formula. Tolerances are not normally specified for four other items, VMA, air voids, Marshall stability, and flow index, probably because the necessary information required does not appear to exist, although the specification limits for each of these four items are expected to be met.
The most generous tolerances from the job-mix formula permitted in North America of which the writer is aware, are those of the American Association of State Highway and Transportation Officials (AASHTO), and of the American Society for Testing and Materials (ASTM), which are identical. The tolerances specified by The Asphalt Institute and by a number of U.S. State Highway Departments are somewhat narrower than those stipulated by ASTM or AASHTO.
The tolerances permitted by AASHTO and ASTM are as follows (1).
Sieve Size -
$4 inch and larger 318 inch and No. 4 sieve No. 8 and No. 16 sieves No. 30 and No. 50 sieves No. 200 sieve
Tolerances Weight Per Cent
of Total Aggregate
f 8.0 2 7.0 f 6.0 'f 5.0 f 3.0
Asphalt content, weight per cent of total paving mixture 5 0.5
If the gradation tolerances should fall outside the specified grading band for a paving mixture, ASTM considers this to be on-specification provided the full grading curve for the job-mix formula itself is within this grading band.
A question that might very naturally be asked about these tolerances is whether or not they are too generous. Since i t is usually an internal matter with most government and other organizations, published inspection data obtained on paving mixtures during their construction are rather scarce. However, some information was published on North Dakota experience by Reich (2) at the 1974 CTAA meeting. Considerable inspection data suitable
Canadian Technical Asphalt Association 1976
for this purpose appear in the paper by Farr, Millions, and Anderson (3) for presentation at this meeting, and inspection data on paving mixtures laid in Saskatchewan in 1975 are available (4). The main value ?? and the standard deviation 0 have been provided for all of these inspection data.
The mean value E plus and minus one standard deviation (E f 0 ), include only 67% of the test values. Consequently, in general, if the specified tolerance limits were based on the mean value E plus and minus one standard deviation, that is on Z 2 8 , 33 per cent of all inspection data would be out- side (either above or below) the tolerance limits. Therefore, in applications of statistics on problems of this kind, it is common practice to base accept- able limits of variation on the mean value Z plus and minus two standard deviations, that is on E 2 2 0 , since these limits cover 95 per cent of all test data.
Using tolerance limits equal to E 2 2 0 , the data for North Dakota published by Reich (1) indicated that the ASTM and AASHTO tolerances are exceeded by a considerable margin at the No. 4, No. 30, and No. 200 sieves, as well as for the paving mixture asphalt contents.
Inspection data listed by Farr, Millions, and Anderson (3) for 73 cold feed analyses for the paving mixture that was laid on Alberta Highway 43, Central Section 22, substantially exceeded the AASHTO and ASTM tolerances at the 318 inch and Nos. 4, 10 and 40 sieves. This is also true for the sieve analysis of aggregates recovered from 18 field extraction tests. The asphalt contents by field extraction on 17 paving mixture samples from this project show variations that are nearly twice the tolerance for asphalt content permitted by ASTM or AASHTO. Even the data for the daily asphalt quantities actually consumed relative to the amount of paving mixtures actually produced each day over a 17-day period, show a variation that materially exceeds the AASHTO and ASTM tolerance for asphalt content.
Inspection data on paving mixtures produced and laid in Saskatchewan in 1975 (4), while demonstrating good aggregate gradation control, show a very wide variation in asphalt content. For 15 out of 18 paving projects, these variations (2 2 (3 ) from the mean value Ti, exceed the 2 0.5 per cent range in asphalt content tolerance permitted by ASTM and AASHTO, and in two cases amounted to a variation (f 2 0 ) in asphalt content of 2.16 and 2.46 per cent, which is more than four times the asphalt content tolerance specified by AASHTO and ASTM.
These are just three examples illustrating the considerable variations in gradation and asphalt content that can occur in asphalt mixtures being placed on actual paving projects. It is suspected that inspection data obtained on numerous paving mixtures being placed elsewhere would show a similar pattern, which could be very much worse on paving projects for which no inspection is being provided. Consequently, the AASHTO and ASTM tolerances, far from being too generous, could provide the target for more effective paving mixture control on a great many paving projects.
The AASHTO and ASTM tolerances are limited to the sieve analyses and asphalt contents of paving mixtures. It is the principal purpose of this paper to present the results of an investigation into the influence that these
Canadian Technical Asphalt Association 1976
ASTM and AASHTO tolerances can have on test values for the five major properties, VMA, air voids, Marshall stability, flow index, and 100 per cent laboratory compacted density, that are associated with sensible paving mixture design.
11: SCOPE OF THE INVESTIGATION
For this investigation, two HL3 and HL6 asphalt paving mixtures were employed. HL3 is a hot-laid surface course paving mixture, Figure 1, and HL6 is a hot-laid binder or base course paving mixture, Figure 2, specified by the Ontario Ministry of Transportation and Communications.
The two HL3 paving mixtures, A-HL3 and B-HL3, differed primarily in that for the A-HL3 paving mixtures, the grading curves for lower-upper and upper-lower, Figure 3, were permitted to be variable with respect to per cent passing the No. 4 sieve. For the B-HL3 paving mixtures, these two grading curves (lower-upper and upper-lower) were required to have the same per cent passing the No. 4 sieve as the corresponding grading curve for the job-mix formula, namely 55 per cent, Table 2. This difference in